Post on 12-Jan-2016
Embed Size (px)
Mathematical Model of Steam Chips and Other Hygroscopic
Drying of Wood Porous Media
Christian Fyhr and Anders Rasmuson Dept. of Chemical Engineering Design, Chalmers University of Technology, S-412 96 Gothenburg, Sweden
A model is presented that is focused on the dying kinetics of single wood chips as a function of time and external conditions, such as temperature, pressure and velocity of the superheated steam. A multiphase and 2 -0 approach was used to model the coupled transport of watec vapor, air and heat in anisotropic hygroscopic porous media. The model was verified by drying experiments where measurements of the average moisture content, center temperature and pressure in a single wood chip could be performed simultaneously. A comparison between the calculations and the measurements showed that the drying behavior was well predicted. The drying can be divided into three stages: a heat-up period when condensation on the surface initially increases the moisture con- tent; a period of constant drying rate when the external heat transfer controls the drying rate; and a period of decreasing drying rate when the drying is controlled by internal mass transfer. Many interesting features of the drying could be assigned to the strong anisotropicity of wood, which makes a 2-0 model necessary.
Introduction Interest in biofuels has increased recently. The main ad-
vantage of these fuels over the fossil ones is that there are no net CO, and SO, emissions. One common form of biofuel is wood chips, which are a by-product of the forest industry. Wood chips stored in piles before drying and combustion, contain about 75% water, on a dry basis, which makes drying necessary in order to achieve effective combustion.
Traditionally the drying medium has been hot air; how- ever, the use of superheated steam is increasing (Wimmer- stedt, 1994). Although the benefits of using this drying medium are mainly economic (reuse of the latent heat of steam), the inert atmosphere also reduces the fire hazards and, since the exhaust steam may be condensed, purification is easier than in the case of air drying.
There are several different types of equipment that are suitable for superheated steam drying. Some examples are the fixed-bed dryer, pneumatic conveying dryer, and fluid-bed dryer. When a pneumatic conveying dryer is used, the drying medium is steam at pressures higher than atmospheric. The pieces of wood are small, so that they can be conveyed by the steam. If the material fed to the dryer is colder than the satu- ration temperature of steam, condensation will occur, which leads to an initial increase in moisture content. The condi-
Correspondence concerning this article should be addressed to A. Rasmuson
AIChE Journal September 1996
tions occurring in a pneumatic conveying dryer will be our main focus. For design purposes, it is of great importance to know how the drying rate of a single particle is affected by the velocity, temperature, and pressure of the superheated steam.
Wood may be considered as a three-phase mixture consist- ing of solid cell walls with liquid water, air, and water vapor filling the lumen spaces. The water exists as free liquid above, and is bound to the cell wall below the fiber saturation point. During the drying process, flow of liquid, gas, and heat oc- curs due to gradients in pressure, water content, and temper- ature. Because of the strong anisotropicity of wood, the mag- nitudes of these flows are very dependent on the direction. This suggests that a multiphase and multidimensional model is required to solve the problem.
A literature search yielded several models for the drying of wood (Spolek, 1981; Plumb et al., 1985; Stanish and Schajer, 1986; PerrC and Degiovanni, 1990). Most of them are focused on one-dimensional air drying of wood planks at atmospheric pressure; only a few are based on fundamental physics. The work presented here is concentrated on the development and experimental verification of a two-dimensional (longitudinal and transversal directions) model and simulation tool that takes into account the most important phenomena present during superheated steam drying of wood chips. The output
Vol. 42, No. 9 2491
of the model is the drying rate as a function of time and external steam conditions as well as internal distributions of moisture, temperature, and pressure. The model is easily generalized to account for air drying. It is envisaged that the model may be used for other hygroscopic materials with ap- propriate specification of material data.
Radiation is modeled according to the Stefan-Boltzman law, where the emissivity for spruce is assumed to be the same as for oak, for which the value 0.9 was found (Perry, 1973).
The most important mechanism for heat transport within a material during drying is conduc- tion, which is modeled according to the Fourier law
Internal Heat Transport.
Transport Processes Drying is a process of simultaneous mass and energy trans-
port occurring both inside and outside the piece of particu- late material. In the case of wood, three moisture phases have to be accounted for: free (liquid) water, bound water, and water vapor. Evaporation rates are determined locally by the interaction of heat flows, temperature changes, and moisture flows.
Moisture in wood can exist in three dif- ferent forms: as free liquid in the cell cavities, Xf, as bound water in the cell walls, X,, or as vapor in the gas phase. Due to the low density of the gas phase, the contribution of vapor to the total moisture content is often disregarded. The boundary between bound and free water is called the fiber saturation point, XFsp, which is dependent on the tempera- ture approximately as (Siau, 1984):
Water in Wood.
XFsp = 0.325 -0.001T. ( 1 )
Equilibrium Moisture Content. Due to the hygroscopicity of wood, an equilibrium between the bound water and the surrounding gas is established. The dependency of this equi- librium of temperature and activity of the steam has been investigated by Bjork and Rasmuson (1995). The sorption forces that hold the water to the cell wall decreases the en- thalpy of the bound water. The heat of sorption is equal to zero at XFsp and increases as the moisture content ap- proaches the equilibrium moisture content. The enthalpy of bound water is then equal to the enthalpy of free water less the enthalpy of sorption, as in the following equation (Stanish and Schajer, 1986):
q = - keffVT (4)
The effective heat-transfer coefficient, keff, is a combination of the heat-transfer coefficients of the three different phases; it is obtained experimentally (Siau, 1984) and is strongly de- pendent on the moisture content. Heat is also transported by convection, as mass transport occurs simultaneously. This is modeled by weighting the mass fluxes with the appropriate enthalpies (see Eq. 11). The ratio of longitudinal to trans- verse thermal conductivity for wood has been found experi- mentally to be approximately 2.5 (Siau, 1984).
For drying in superheated steam, there is no resistance to mass transfer present at the surface. The convective transport of vapor across the surface equal- izes the pressure between the surface and surroundings. The model can easily be extended to take external resistance for mass transfer into account (i.e., air drying). This can be ac- complished by inserting a convective mass-transfer expression similar to the external heat transfer at the surface.
Internal Mass Transfer. The two-phase flow of fluids through porous media is described by an extended Darcys law (Dullien, 1979)
External Mass Transfer.
where n is the flux, K is the saturated permeability, k , the relative permeability, and p the viscosity of phase a. The gravitational term, g, may be disregarded in vapor flow due to the small value of the density. The relative permeability is dependent on the saturation and on the porous material. In wood, flow of liquid occurs only above the fiber saturation point, where free liquid is present. The gaseous phase is mo- bile at all moisture contents except near full liquid satura- tion. For an anisotropic medium such as wood, the relative permeability becomes a tensor of the second order. Typically, the ratio K,/K, is of the order lo3 for softwood (Siau, 1984). The pressures in each phase are coupled through the rela- tion:
External Heat Transfer. Heat is transferred from the sur- rounding steam to the surface of the wood chip by convec- tion. Since the fluid stream impinges on the edge, small vor- tices may form just behind the leading edge, due to the finite thickness of the chip. Sorensen (1969) investigated the mass- transfer coefficients of truncated slabs and obtained the fol- lowing correlation (expressed in heat transfer terms). Pg - PI = P,, ( 6 )
h (3) where P, is the capillary pressure that arises from surface tension effects at the liquid-gas interphase.
In addition to flow, diffusive transport of both the gaseous
S t = - - - - - 0.152ReE.179[Rex -49.8ReE.61]-o.5 P ucp
250 < Reb < 16,000 2 < Re, < lo5. and liquid phases may take place. Gaseous diffusion is negli- gible in the case of steam drying but may be of importance in air drying. Bound water is mobile due to surface diffusion effects (Skaar and Babiak, 1982), and the transport of bound water is modeled according to Ficks law:
The blunt edged plate expression predicts higher local heat-transfer coefficients close to the edge than the ordinary expression for flat plates. This is explained by turbulence production as the flow passes by the edge of the truncated slab. It = - DswVX (7 )
2492 September 1996 Vol. 42, No. 9 AIChE Journal
where n is the mass flux due to diffusion, V X